Advances in Electrical Engineering
Volume 2014 (2014), Article ID 423803, 5 pages
http://dx.doi.org/10.1155/2014/423803

Research Article

Proton Irradiations on SJ HV Power MOSFETs to Realize Fast Diode Devices

Ignazio Bertuglia, Giuseppe Consentino, and Michele Laudani

Power Transistors Division, STMicroelectronics, Catania, Italy

Received 4 June 2014; Revised 31 July 2014; Accepted 19 August 2014; Published 3 November 2014

Academic Editor: Changhwan Shin

Copyright © 2014 Ignazio Bertuglia et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.

Abstract.

This paper studies the effects of proton irradiations on Super Junction High Voltage power MOSFETs to realize transistors with fast diode. Experiments were performed on a sample of 600 V power MOSFETs and achieved results were compared to standard irradiated devices by electrons.

1. Introduction

In many modern applications and, in particular, when using full bridge converters, intrinsic diode of HV power MOSFET is even utilized to free wheel the current in the circuit without using any other external component [1–7]. Intrinsic diode of a power MOSFET is implemented by considering the body-drain junction of the same device. In fact, when the device is switched off and the transistor is polarized in reverse mode, the current flows from the source to the drain terminals working in third quadrant configuration. In such operating conditions, intrinsic diode needs to guarantee particular performances and features. In particular, diode needs to be fast in order to reduce switching losses when operating switching frequencies increase. A diode becomes fast when charges moved during rapid variation of against time are quite low as shown in Figure 1. In fact, in the example shown in Figure 1, MOSFET is rapidly switched off. When increases, drain current decreases down to negative values because charges stored in the body-drain junction need to be discharged. Standard devices (red curve) reach the lowest peak of drain current () because the charge stored in the junction () is higher than fast devices (green curve). That turns in a higher time to discharge () and, thus, it makes the devices slower during commutation. To improve the performances of intrinsic diode, special processes need to be implemented. The typical action consists in the irradiation of the body-drain junction by energetic electrons in order to create suitable damage in the reticle. Such damage introduces deep energetic level traps in the silicon band-gap. Such traps capture the carriers lowering the quantity of charges moved during the fast transition from on to off states as described above. Typical irradiation doses are in the range of 5–50 MRad when considering power MOSFETs. Afterwards, a thermal process needs to be implemented in order to activate the traps. However, irradiation by considering electrons can bring issues related, for example, to the quality of gate oxide. In fact, interface traps states can be created increasing drain-source leakage current.

Figure 1: Example of commutation of the intrinsic diode and comparison with a fast diode.

Recently, a new technique was implemented to realize devices with fast diodes based on proton irradiation. In fact, protons can be introduced in the body-drain junction of a power MOSFET’s structure only concentrating the effect on the body-drain border junction differently from the electrons which are implanted on the entire structure.

2. Protons Irradiation, Experiment Setup, and Test Vehicles

A series of experiments were implemented by changing the dose of protons irradiation and acting on thermal process to evaluate the best solution and to compare the results with the standard electron irradiation process. The tests were performed by considering a tandem accelerator with protons at energies in the ranges of some MeV useful to reach the depth inside of body-drain junction of the devices. The irradiation has been performed in air where at 1 cm of distance is located the wafer under test. Wafers were mounted on a frame connected to a precise step by step motor utilized to move it. To perform these experiments, a family of SJ HV power MOSFETs of 600 V was considered (see in Table 1 the peculiarities of the adopted test vehicle). Typical cross section of a Super Junction device is shown in Figure 2 where the depth of implant is even highlighted.

Table 1: Main characteristics of test vehicle.

Device type
SJ HV power MOSFETs used

BVdss [V]
continuous @ 25°C [A]
[V]

n-ch
600
35
4

Figure 2: Example of cross section of a Super Junction HV power MOSFET. (1) Gate planar oxide; (2) body region; (3) EPY drift region; (4) back-drain contact; (5) source well-source contact; (6) polysilicon; (7) current flow; (8) metal; (9) drain column; and (10) region to be damaged by proton.

Irradiation of protons was implemented either in the front or in the back side of the wafer considered, reaching different depths in the region included between the body-drain junction and the same epitaxial layer under the pillars. Based on simulation activity, it was established that fluency of protons on the silicon needs to be in the range of 10¹¹ cm⁻² and  cm⁻² in order to compare with effects of electrons in silicon. It is necessary to observe that protons’ irradiation implies a certain tail of damage along the initial path of the trajectory that could affect the electrical performances of the devices. For example, if the implantation is performed by the top of the wafer, the tail of damage involves essentially the first micrometers of silicon layers in the top of the die. Such vacancies could even affect the reliability of the gate oxide. These considerations will be more evident after studying the experimental results on the wafer irradiated on the front of the wafers. After the proton implantations, wafers under tests were thermally treated in furnaces and, afterwards, they finished the process (back end). Before packaging the dices, wafers were tested to evaluate the performances in terms of (diode recovery time), (diode recovery charge), and (reverse peak current during the recovery time of diode). Figure 3 and Tables 2, 3, 4, and 5 report the data when a polarization which equals 60 V is applied.

Table 2: Main results on wafer bench—implantation on the front EPI layer.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]
BVdss [V]

5 * 10¹²
5.1
120
354
500

1 * 10¹²
9.2
189
936
610

5 * 10¹¹
11.5
237
1466
650

1 * 10¹¹
21.1
400
4475
680

No irradiation
29.6
534
7582
680

Std. electrons
8.7
184
877
660

Table 3: Main results on wafer bench—implantation on the front body-drain junction.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]
BVdss [V]

5 * 10¹²
6.7
180
602
460

1 * 10¹²
9.7
242
1176
570

5 * 10¹¹
12.5
308
1926
630

1 * 10¹¹
19.1
474
4524
670

No irradiation
29.6
534
7582
680

Std. electrons
8.7
184
877
660

Table 4: Main results on wafer bench—implantation on the back body-drain junction.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]
BVdss [V]

5 * 10¹²
7.7
194
747
490

1 * 10¹²
10.9
271
1475
600

5 * 10¹¹
14.1
343
2421
640

1 * 10¹¹
17.3
427
3692
680

No irradiation
29.6
534
7582
680

Std. electrons
8.7
184
877
660

Table 5: Main results on wafer bench—implantation on the back EPI layer.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]
BVdss [V]

5 * 10¹²
9.5
232
1108
630

1 * 10¹²
11.9
282
1678
660

5 * 10¹¹
13.5
335
2262
670

1 * 10¹¹
19.1
477
4550
680

No irradiation
29.6
534
7582
680

Std. electrons
8.7
184
877
660

Figure 3: Example referred to data of Table 3.

As it is possible to see from the above data, by increasing proton dose , , and decrease and the diode switching performances improve. However, results are different if compared to several trials and with standard irradiated devices with electrons. In fact, considering the devices irradiated around the body-drain junction with a concentration of 10¹² cm⁻², is comparable to standard irradiated transistors. Instead, considering devices with an implanted dose of  cm⁻², is lower than standard irradiated transistors. Considering devices irradiated in the epitaxial region with a concentration of  cm⁻², is quite similar to standard one. It is necessary to highlight that when the dose increases, a lowering of breakdown voltage is observed together with an increasing of drain-source leakage currents. Such results are more evident when dice implanted from the top are considered. This phenomenon can be explained taking into account that tails of the damage, located near the body-drain junction, change the charges balance inside the space charge region.

Comparable results can be achieved by considering packaged devices when current is switched off at around 27 A (different operating condition compared to the previous test). In Tables 6–9 and Figures 4, 5, 6, and 7 data regarding dynamic measurements of packaged devices are shown.

Table 6: Main results on packaged power MOSFETs—implantation on the front EPY layer.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]

5 * 10¹²
13
162
1180

1 * 10¹²
18
203
1870

5 * 10¹¹
24
267
3460

1 * 10¹¹
36
448
8612

Std. electrons
18
180
1800

Table 7: Main results on packaged power MOSFETs—implantation on the front body-drain border.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]

5 * 10¹²
10
116
630

1 * 10¹²
19
233
2370

5 * 10¹¹
23
254
3133

1 * 10¹¹
35
414
7626

Std. electrons
18
180
1800

Table 8: Main results on packaged power MOSFETs—implantation on the back body-drain border.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]

5 * 10¹²
18
190
1756

1 * 10¹²
20
228
2410

5 * 10¹¹
26
286
4056

1 * 10¹¹
34
406
7400

Std. electrons
18
180
1800

Table 9: Main results on packaged power MOSFETs—implantation on the back EPY layer.

Dose [cm⁻²]
SJ HV power MOSFETs results

[A]
[ns]
[nC]

5 * 10¹²
19
205
2058

1 * 10¹²
23
253
3110

5 * 10¹¹
27
290
4200

1 * 10¹¹
35
431
8330

Std. electrons
18
180
1800

Figure 4: Example referred to data of Table 6.

Figure 5: Example referred to data of Table 7.

Figure 6: Example referred to data of Table 8.

Figure 7: Example referred to data of Table 9.

3. Conclusions

This paper has analyzed the effects on SJ HV power MOSFETs of proton irradiations to realize intrinsic “fast diode” components. Intrinsic diode needs to be fast in order to decrease switching losses and to increase operating switching frequencies without any issue related to dV/dt. In order to improve the performances of intrinsic diode, typical action consists in the irradiation of the body-drain junction by energetic electrons. Electronic irradiations can sometimes bring issues related, for example, to the quality of gate oxide because they are spread out in the entire wafer volume. Instead, protons are localized in a specific part of the die and, in particular, in the epitaxial layer slightly below the body-drain junction. A series of experiments was performed by considering a suitable proton irradiator on samples of Super Junction High Voltage power MOSFETs with a breakdown voltage of 600 V. Irradiations with protons were implemented either in the front or in the back side of the wafers with projected range in the region between the body-drain junction and the same epitaxial layer under the pillars. Based on simulations, it was established that fluency of protons on the silicon needs to be in the range of 10¹¹ cm⁻² and  cm⁻² to compare with effects of electrons irradiation on silicon. After the proton implantations, wafers under tests were thermally treated by considering dedicated process flow. Therefore, several measurements were performed either considering tested dice on wafers or considering static and dynamic characterizations after the packaging. Experimental results show that , , and decrease by increasing proton doses. However, it is necessary to highlight that when the dose increases, a lowering of breakdown voltage is observed together with an increasing of drain-source leakage currents.

Therefore, it is possible to assume that the best trial, in terms of reverse recovery performance, was the one with protons implanted on the back side with a dose of  cm⁻². Nevertheless, breakdown voltage degradation implies that a more optimized solution still has to be found by investigating different doses combined with thermal annealing process fine tuning, just to improve performances without BV degradation.

Conflict of Interests

The authors declare that there is no conflict of interests regarding the publication of this paper.

References

P. Hazdra, J. Vobecký, and K. Brand, “Optimum lifetime structuring in silicon power diodes by means of various irradiation techniques,” Nuclear Instruments and Methods in Physics Research B: Beam Interactions with Materials and Atoms, vol. 186, no. 1–4, pp. 414–418, 2002.

J. Lutz, R. Siemieniec, F. J. Niedernostheide, and H. J. Schulze, “Characteristics of irradiation induced deep levels in silicon,” in Proceeding of the Solid State Chemistry and Modern Micro- and Nanotechnologies Conference, Kislovodsk, Russia, 2005.

M. Schmitt, H.-J. Schulze, A. Schlogl et al., “A Comparison of Electron, Proton and Helium Ion Irradiation for the Optimization of the CoolMOSTM Body Diode,” Infineon Technologies AG, AI PS DD, Balanstr. 59, D-81541 Munich, Germany, 2011

V. Benda, “Design considerations for fast soft reverse recovery diodes,” in Proceedings of the 15th European Conference on Power Electronics and Applications, Brighton, UK, September 1993.

P. Lévêque, P. Pellegrino, A. Hallén, B. G. Svensson, and V. Privitera, “Hydrogen-related defect centers in float-zone and epitaxial n-type proton implanted silicon,” Nuclear Instruments and Methods in Physics Research, Section B: Beam Interactions with Materials and Atoms, vol. 174, no. 3, pp. 297–303, 2001.

T. Mizushima, M. Nemoto, H. Kuribayashi, T. Yoshimura, and H. Nakazawa, “Inhibiting effect of middle broad buffer layer diode using hydrogen-related shallow donor on reverse recovery oscillation,” in Proceedings of the 22nd International Symposium on Power Semiconductor Devices & IC's (ISPSD '10), pp. 115–118, June 2010.

R. Siemieniec, F.-J. Niedernostheide, H.-J. Schulze, W. Südkamp, U. Kellner-Werdehausen, and J. Lutz, “Irradiation-induced deep levels in silicon for power device tailoring,” Journal of the Electrochemical Society, vol. 153, no. 2, pp. G108–G118, 2006.